Electrooxidation of methanol on carbon supported pt ru nanocatalysts prepared by ethanol reduction method
Int. J. Electrochem. Sci., 6 (2011) 379 - 393 International Journal of ELECTROCHEMICAL SCIENCE www.electrochemsci.orgElectrooxidation of Methanol on Carbon Supported Pt-Ru Nanocatalysts Prepared by Ethanol Reduction MethodA. B. Kashyout1,*, Abu Bakr A.A. Nassr1, 2, Leonardo Giorgi2, T. Maiyalagan3,Bayumy A. B. Youssef 41 Electronic Materials Department, Advanced Technology and New Materials Research Institute,Mubarak City for Scientific Research and Technology Applications, 21934 New Borg El-Arab City,Alexandria, Egypt.2 ENEA, Casaccia Research Centre, Department of Physical Technologies and New Materials, ViaAnguillarese 301, 00123 S. Maria di Galeria, Rome, Italy3 Department of Chemistry, VIT University, Vellore-632014, India4 Department of Computer Based Engineering Applications, Informatics Research Institute, MubarakCity for Scientific Research and Technologies Applications, 21934 New Borg El-Arab City,Alexandria, Egypt* E-mail: firstname.lastname@example.orgReceived: 26 January 2010 / Accepted: 1 December 2010 / Published: 1 February 2011Carbon Supported PtRu nanocatalysts have been prepared by simple impregnation reduction method inwhich Pt and Ru precursors are reduced by ethanol under reflux conditions for different reaction times.The prepared nanocatalysts were characterized by means of XRD, EDAX, ICP-AAS, FESEM andTEM. XRD analyses showed that all nanocatalysts exhibited f.c.c crystal structure, the structurecharacteristic for pure Pt, except for that reduced at prolonged reaction time of 4h which showed thepresence of characteristic peak for Ru metal. The lattice constant calculations indicate that all catalystsare present in unalloyed phase and the average particle size as determined by TEM was in the range of3.7 nm. The electrocatalytic activities and stability for the prepared nanocatalysts methanol electro-oxidation reaction (MOR) were studied by cyclic voltammetry. The catalysts prepared at 2h reductiontime showed higher electrocatalytic activity in terms of mass specific activity and good stability overpotential sweep for 100 cycles for methanol electro-oxidation. The results showed that the preparednanocatalysts are considered as promising electrode catalyst (anode catalyst) for electro-oxidation ofmethanol in direct methanol fuel cells.Keywords: PtRu nanocatalysts, methanol electro-oxidation, cyclic voltammetry, DMFCs
Int. J. Electrochem. Sci., Vol. 6, 2011 3801. INTRODUCTION The electro-oxidation of small organic molecules on Pt electrocatalysts based electrodes hasreceived more attention in the last decades due their application for electrochemical energy conversionin direct liquid feed fuel cells [1-3]. Among these molecules; methanol is used as liquid fuel for directmethanol fuel cells (DMFCs). It has a higher electron density (six electron production during itselectro-oxidation) and it has a good electrochemical activity due to the presence of electroactivehydroxyl group which can be attached or adsorbed to the electrode surface . The electro-oxidation of methanol has been studied on many electrode fabricated fromunsupported metals and metal supported onto different supporting materials. Pt catalysts are still themost active catalysts materials for electro-oxidation of methanol [3, 5-9]. The electro-oxidation ofmethanol on Pt electrode surface is combined with several steps of dehydrogenation to form CO whichis oxidized into CO2 [10, 11]. The poisoning of the electrode surface (anode) by CO molecules formedduring the methanol oxidation is one of the obstacles in the development of DMFCs for commercialapplications. The modification of Pt catalysts with other metals or metal oxides which have highertendency to form surface oxygenated species at lower potential is considered as one of the best ways tosolve this problem [12, 13]. In this regard, many efforts have been done by many groups to synthesisnew catalysts systems for methanol oxidation based on bimetallic catalysts such as PtRu[14-17],PtSn[18,19], PtNi[20,21], PtMo[22,23],ternary alloy ; PtRuNi[24-26], PtRuMo[25,27,28], and PtMOx(where M is, Ti, V, Mn, W) [29-32]. Among all catalyst systems, PtRu catalysts prepared as nanoparticles have received moreattention due to its high CO tolerance. The formation of surface oxygenated species on Ru takes placeat a potential lower than that on Pt. So, the presence of Ru adjacent to Pt reduces the poisoning of Ptsurface by CO [8,9]. In this catalyst system, Pt services as active sites for methanol adsorption anddehydrogenation while Ru serves as catalyst promoter on which CO is oxidized into CO 2. This modelmechanism is known as bifunctional mechanism. Other model is suggested based on electronicstructure change upon addition of Ru. According to this model, the addition of Ru can change theelectronic structure of catalyst surface which lead to decrease the bonding between the CO moleculesand Pt catalyst surface [8, 9, 33]. Many research groups are working to explore preparation method for PtRu catalyst system .The catalytic activity of the catalysts depends on their preparation methods. Also, the cost of catalystspreparation process should be taken into consideration for the application in fuel cells. Therefore; thesearching for simple preparation methods with low cost and high catalytic activity will lead to thedevelopment of fuel cells industry. Wet chemical method or some times called chemical impregnation method is considered as themost powerful method for preparation of catalysts nanoparticles specially; supported PtRu catalysts.The procedures for this method are easy and can be developed for large-scale production [7, 34]. Inwet chemical method, the metal precursors are impregnated on the carbon support in aqueous or/andorganic media followed by the reduction using reducing agent such as sodium borohydride, formicacid, hydrazine. Also, the organic alcohols (methanol, ethanol, isopropanol and ethylene glycol,glycerol and diethylene glycol) are known as good reducing agents for the preparation of PtRu and
Int. J. Electrochem. Sci., Vol. 6, 2011 381other nanoparticles. Advantages of using alcohols as reducing agent are that there is no side reactionproducts can be obtained and the formation of relative pure nanoparticles are well synthesized[7,34,35]. The reduction process are carried out in presence of stabilizers such as PVA or other polymersor surfactant materials which serve as capping agent to prevent the particle agglomeration. In fact,these capping materials have adverse effect on the electrocatalytic activity, since these stabilizers areadsorbed on the surface of the nanoparticles catalysts and blocking the active sites available for theelectrochemical reaction in addition to its lower electrical conductivity. Also, the removal of theseprotective agents by heat treatment may be has side-effect on the electrocatalytic activity due thechange of crystal structure of the active phase in the catalysts or increase their particle size [36, 37]. Lee e.t al. prepared PtRu/C nanocataysts using ethanol reduction method and tested theprepared catalysts for methanol electooxidation reaction . The results showed that the preparationprocess has adverse effect on the electrocatalytic activity when carried out in alkaline media. Also,carbon supported Pt and PtAu catalysts as electrocatalysts for oxygen reduction reaction (ORR) havebeen prepared by ethanol reduction method in the presence of PVP as stabilizing and complexingagent. The reduction process were carried out in alkaline media. The removal of the stabilizing agentwas carried out by heating the catalysts at high temperature in air followed by their reduction in flowof hydrogen at elevated temperature. The prepared electrocatalysts showed good electrocatalyticactivity towards ORR . In this work, we report a simple method for preparation of PtRu nanoparticles supported oncarbon support (Vulcan XC-72R) by using ethanol as a reducing agent without using any stabilizersand no modification of the preparation media (pH) and without heat treatment. The preparednanocatalysts are characterized by means of structural tools; XRD, FESEM and TEM and chemicalanalyses by EDAX and ICP-AAS. The electrocatalytic activity is tested for methanol electrooxidationby cyclic voltammetry technique. The effect of reduction time on the durability of the catalysts is alsostudied.2. EXPERIMENTAL PART2.1. Electrocatalyst Preparation In this work, a carbon supported PtRu nanoparticles electrocatalyst with atomic ratio Pt:Ru(1:1) and 20% wt of metal loading (PtRu) on carbon was prepared according to the followingprocedures. 100 mg of carbon (Vulcan XC-72R) was dispersed in 20 ml ethanol in an ultrasonic bathfor 15 min. To the above suspension; 34.6 mg of H2PtCl6 dissolved in 5 ml water and 17.5 mg ofRuCl3 dissolved in 5 ml of water were added and then 80 ml of ethanol was also added to the reactionmixture. The total mixture was kept under stirring for 1h followed by sonication in an ultrasonic bathfor 30 min to insure the adsorption and dispersion of the metal precursors on the carbon support. Theresulted mixture was heated under reflux at (80 ± 2°C) under stirring for different reaction times afterwhich the reaction mixture was leaved to cool to room temperature and then centrifuged to separate the
Int. J. Electrochem. Sci., Vol. 6, 2011 382catalysts powder. The catalysts were subjected to many cycles of washing with water and centrifugeuntil no Cl – ions were detected (silver nitrite test) and then dried in vacuum oven at 100°C for 12h. The reductive reactions can be represented by the following equations : H2PtCl6 + 2C2H5OH → Pt + 2 CH3CHO + 6 HCl 2RuCl3 + 3C2H5OH → 2Ru + 2 CH3CHO + 6 HCl The PtRu/C catalysts produced during this work are (PtRu/C1, PtRu/C2 and PtRu/C4). Theselabels are giving according to their reaction times of 1h, 2h and 4h; respectively.2.2. Electrocatalyst Characterization2.2.1. Physical and Chemical Characterization The total metal loading was determined by ICP-AAS (Prodigy, high dispersion ICP, Leman).The measurement was carried out by collecting all the filtrates during the washing process anddetermining the concentration of Pt and Ru contents in the filtrate from which we can calculate theamount of metal loading on the carbon support. The chemical composition of the prepared catalystswas determined by the energy dispersive X-ray analysis (EDAX) combined with SEM (JEOL JSM6360LA). X-ray diffraction study of the prepared nanocatalysts were carried out using (Schimadzu7000) diffractometer, operating with Cu Kα radiation (λ=0.154060 nm) generated at 30 kV and 30 mAwith scanning rate of 2º min-1 for 2θ values between 20 and 90º degree. The nanocatalysts morphologyand dispersion on the support and their particle size were investigated by FESEM (LEO 1530) andTEM (JEOL, 200CX). The samples were prepared by dispersion of the catalysts powder in ethanol andsonication, then the sample was deposited on a diamond polished graphite paper supported onaluminum sample holder for FESEM analysis and on carbon coated Cu grid for TEM analysis. The average particle size and particle size distribution are acquired using FORTRAN code. Thecode has been made to apply the image processing rules on the TEM images of PtRu/C catalysts todetermine exactly the average particle size and the particles size distribution from digital images. The code design steps are removing the background (the carbon support), clustering the pixelswhich form each particle and finally computing the diameter of each particle . Removing ofbackground has been done using the threshold technique. For clustering of the pixels; the clusteringbased iterative method has been used. The method mainly depends on getting certain relation betweeneach pixel and its neighbors. This relation is applied iteratively until the results of this relation have novariation with increasing the iteration:1. Starting with two arrays (A, B) which have a number of elements. Each element is corresponding to each pixel of image.
Int. J. Electrochem. Sci., Vol. 6, 2011 3832. Fill the arrays A and B with large number. This number must be greater than the expected particles number (LN)3. Putting a variable N as counter for particle Number4. Starting N=05. Calculating every array elements according the next relation: Bi , j Min( Ai 1, j , Ai 1, j , Ai , j 1 , Ai , j 1 )6. If Ai , j is equal to the larger number LN then N N 1 and Ai , j N7. If Ai , j is less than (LN) , Ai , j remains unchanged8. Getting r A B9. If r equal zero the solution is accomplished if not the program must execute steps 5,6,7,8,9 after putting A B Finally, the array A contains the particle numbers corresponding to all pixels of the image.From the total number of pixel we calculated the area of each particle which subsequently used tocalculate the particle size.2.2.2. Electrochemical Measurements The electrocatalytic activities of the prepared catalysts were evaluated towards methanolelectrooxidation reaction (MOR) in a standard three electrodes electrochemical cell in which staturedcalomel electrode (SCE) (0.241 vs. NHE) and high purity graphite electrode were used as referenceelectrode and counter electrode; respectively. The working electrode is glass carbon disc (GCD)electrode coated with the catalyst layer. The catalysts layer was prepared by mixing the catalystpowder with Nafion solution (10% Wt , DuPont), water and isopropanol and then sonicated inultrasonic water bath for 15 min followed by magnetic stirring for1h to form a catalyst ink whichfinally coated on GCD and dried for 20 min at 80 ºC. The working electrode area was 0.79 cm2 and theamount of catalysts loading (PtRu in mg/cm2) in the working electrode was controlled to be 0.2mg/cm2. The measurements were carried out with EG&G 273A potentiostat/galvanostat fromPrinceton Applied Research (PAR) and controlled with Corware/Corview software (ScribnerAssociates). The electrode measurements were activated in 1M H2SO4 by sweep the electrode between-0.28 – 1 V (SCE) with a scan rate of 100 mVs-1 till the reproducible voltammogram was obtained(about 100 cycles). The electrocatalytic activity for methanol electro-oxidation was tested in 0.5 MCH3OH/1 M H2SO4 solution in the same potential window and at the same scan rate. Before theelectrochemical measurements, the cell was bubbled with N2 gas for at least 20 min and the N2 gasflow was maintained over the solution surface during the measurements. All chemicals during this
Int. J. Electrochem. Sci., Vol. 6, 2011 384work were an analytical reagent grade and the solutions were prepared from distilled water. Themeasurements were carried out at room temperature.3. RESULTS AND DISCUSSION3.1. Physical and chemical characterization3.1.1. Chemical composition analysis Metal atomic composition (Pt:Ru, atomic ratio) and weight percent determined by EDAX andthe ICP are shown in Table (1). Pt:Ru is very closed to 1:1 atomic ratio which agrees with the nominalconcentration of Pt and Ru in the starting precursor. During the EDAX analysis, no peaks for Cl or Nawere observed, which insure that these undesirable elements were removed during the washingprocess. On the other hand, ICP analyses showed that the PtRu loading was 18 wt% for all catalystswhich is near to the starting loading percentage of 20 % and confirms that almost all the Pt and Ru ionsare reduced to their corresponding metallic state.Table 1. Chemical composition of PtRu/C catalysts from EDAX and ICP-ASS AnalysesCatalysts Type Reaction time At % (from EDAX) Wt % (From ICP-Ass) hr Pt Ru Pt Ru PtRu/C1 1 47.59 52.41 11 7 PtRu/C2 2 48.05 51.95 11 7 PtRu/C4 4 45.11 54.89 11 73.1.2. X-ray diffraction Fig.(1) shows the X-ray diffraction patterns for the prepared catalysts, e.g. PtRu/C1, PtRuC2and PtRuC3 respectively. X-ray diffraction analyses show that all catalysts exhibit the diffractionpeaks of (111), (200), (220) and (311), respectively.Table (2): Diffraction peaks for PtRu/C catalysts and pure Pt with their corresponding 2θ valueCatalysts Type (111) (200) (220) (311) Pure Pt 39.7º 46.2º 67.4º 81.2º PtRu/C1 39.8º 46.2º 67.8º 81.6º PtRu/C2 39.8º 46.2º 67.7º 81.6º PtRu/C4 39.9º 46.1º 67.8º 81.6º These peaks are the characteristic for Pt face-centered cubic structure (f.c.c) (JCPDS Card No.04-802). The wide peak near 2θ = 25° corresponds to the diffraction of the carbon support (Vulcan
Int. J. Electrochem. Sci., Vol. 6, 2011 385XC-72R). The diffraction peaks are located approximately at nearly 2θ values as that of pure metallicPt as shown in Table 2. Since there is no shift of the diffraction peaks for higher 2θ value than that ofpure Pt, no alloys formation or solid solution between Pt and Ru in the prepared PtRu/C can bedetected which is in agree with the results of lattice constant calculated for all the prepared catalysts(Table. 3) . 350 (111) (PtRu/C4) (200) (220) (311) Intensity (a.u) (PtRu/C2) (PtRu/C1) 20 30 40 50 60 70 80 90 2 (Degree) Figure 1. XRD patterns for PtRu/C catalysts prepared at different reaction time. For the catalysts PtRu/C1 and PtRu/C2, there are no diffraction peaks characteristic forRu or its oxide, even with the smooth profile obtained after elimination of the back ground and highfrequency noise by the instrumental software. The same results are reported by many groups forPtRu/C catalysts [41-43] and this may be attributed to Pt that is decorated by Ru particles or may beRu is present in amorphous phase or in form of hydrous Ru-oxide [43-46]. For PtRu/C4 catalyst, thereis a new low intensity diffraction peak at about 2θ =44° between those of Pt (111) and (200). The peakwas detected from the smooth profile of XRD pattern for PtRu/C4. This peak is the characteristic for(101) diffraction plane of Ru, most intense reflection plane for h.c.p Ru . This suggests that inPtRu/C4, Ru is presence as a separate phase. The particle size for all the prepared catalysts is calculated from the width of (220) diffractionpeak using Gaussian fitting using Scherer equation [42,43,47]: 0.95 D 2 cos max Where D is the particle size in (nm), λ is the wave length (0.15406 nm), β2θ is the fullwidth athalf maxima in radius and θmax is the angle at high maxima.
Int. J. Electrochem. Sci., Vol. 6, 2011 386 The lattice constant for the prepared catalysts was calculated from (220) diffraction peak byusing Bragg law according to the following equation [42, 43]: 2 a fcc sin The particle size and the lattice constant for all prepared catalysts are given in Table (3). For allthe prepared catalysts, the calculated particle size is nearly equal to about 3.7 and 3.8 nm whichindicates that the particle size is slightly influenced by the reaction time. Also, the lattice constants for all the catalysts are much closed to that of pure Pt which confirmsthat PtRu catalysts are present in unalloyed form. The relative crystallinity of the prepared catalysts can be calculated from the ratio between theheight peak of Pt (111) and peak reflection of the carbon. These values of relative crystallinity aregiven in Table (3). From Table (3), catalysts PtRu/C2 has a higher crystallinity than that of PtRu/C1and PtRu/C4.Table 3. The structural parameters for PtRu/C catalysts from XRD analysis and average particle size from TEM calculations.Catalysts type Particle size Lattice constant Relative crystallinity Average particle size XRD (nm) (nm) TEM (nm)PtRu/C1 4.9 0.3906 4.85 3.7PtRu/C2 4.9 0.3908 5 3.7PtRu/C4 4.7 0.3906 3 3.8PtRu/C . - - - 6.963.1.3. FESEM and TEM analysis Fig (2) and Fig (3) show the FESEM and TEM images of the synthesized PtRu/C catalysts.From both FESEM and TEM images we observe the deposits of PtRu nanoparticles on the carbonsupport. The nanoparticles are in good dispersion on the support. For PtRu/C4, the presence of large amount of agglomeration is observed and some of thecarbon particles were not covered by PtRu nanoparticles. The histograms for particle size distribution are shown in Fig (3). The average particle sizeswere 3.7, 3.7, 3.8 for PtRu/C1, PtRu/C2, PtRu/C4; respectively. The average particle for PtRu/C catalysts reported in this work is smaller than that reported byLee et al using the same preparation method, which was 6.96 nm and 10.2 nm upon addition of 1MNaOH. 
Int. J. Electrochem. Sci., Vol. 6, 2011 388 30 Particle size =3.7 25 S.D.= 1.1 Frequency % 20 15 10 5 0 2.5 3 3.5 4 4.5 5 5.5 6 Particle size (nm) 30 Particle Size =3.7 25 S.D.= 0.96 Frequency % 20 15 10 5 0 2.5 3 3.5 4 4.5 5 6 Particle size (nm) 25 Particle size =3.8 S.D.= 1.05 20 Frequency % 15 10 5 0 1 2 3 4 5 6 7 8 Particle size (nm)Figure 3. TEM photographs for PtRu/C catalysts (PtRu/C1;(a), PtRu/C2; (b), PtRu/C4; (c)) and the corresponding histograms.3.2. Electrochemical measurements The cyclic voltammograms for PtRu/C catalysts in H2SO4 are shown in Fig (4, column A). ThePtRu/C1 and PtRu/C4 showed the typical behavior of Pt electrode in H2SO4 with peaks in hydrogen
Int. J. Electrochem. Sci., Vol. 6, 2011 389adsorption-desorption region (-0.2– 0.15 V vs. SCE) and a peak for PtOx reduction in the reverse scan.The characteristic peaks were well defined in case of PtRu/C1 than that on PtRu/C4. It appears fromthese characteristics that the two catalysts have Pt-rich surface. On the other hand, for PtRu/C2, the H-desorption peaks are very low and the peak for PtOx is suppressed completely. It is reported that thebehavior of Pt catalyst electrode in H2SO4 is affected by the incorporation of Ru and its percent on thesurface and PtRu catalysts with 50 At. % doesnt show the same behavior of Pt catalysts. Thesuppressed of hydrogen desorption process in PtRu/C2 may be attributed to the formation RuOx atlower potential and it could be due to the presence of hydrous Ru-oxide . The CV’s for methanol oxidation on all prepared catalysts electrodes are shown in Fig (4,column B). All cyclic voltammograms are similar to methanol oxidation voltammograms reported inthe literature [32, 46], with the peak for oxidation of methanol in the forward scan and another peak inbackward scan characteristic for oxidation of intermediate adsorbed on the electrode surface in theforward scan. For the PtRu/C4, the peak potential for methanol oxidation is shifted for higher potentialthan that of other catalysts. This may be attributed to the agglomeration of nanoparticles catalysts as itdetected by FESEM and TEM. The high dispersion and uniform distribution of nanoparticles catalystsin the carbon supports could enhance the electrocatalytic activity of the nanocatalysts. Theelectrocatalytic activities for all the catalysts are evaluated using mass specific activity (MSA) andpeak potential for methanol electrooxidation. The MSA was calculated by integration of the chargedensity corresponding for methanol oxidation divided by metal loading according to the followingequation [48-50]: Q MSA MOR LPtRu Where the MSA is the mass specific activity for MOR (mCmg-1), QMOR is the charge densityfor methanol oxidation peak (mC/cm2) and LPtRu is the loading of PtRu in the electrode (mg/cm2) The values for mass specific activities for all catalysts electrodes at steady state (after 50cycles) and the peak potential for methanol electrooxidation are shown in Table (4).Table 4.Mass specific activities for PtRu/C catalystsCatalysts type MSA (mCmg-1) CH3OH oxidation peak potential (V) PtRu/C1 175 0.69 PtRu/C2 196 0.68 PtRu/C4 165 0.75PtRu/C2 showed higher MSA which indicates that the electrode fabricated from this catalyst hashigher electrocatalytic activity towards methanol electro-oxidation reaction. This higherelectrocatalytic activity of PtRu/C2 could be attributed to high dispersion or more homogenous ofnanoparticles catalysts on the support and the formation of hydrous ruthenium oxide. It is reported thatthe hydrous ruthenium oxide has promoter effect in PtRu catalysts more than that the Ru alloyed inPtRu 
Int. J. Electrochem. Sci., Vol. 6, 2011 390 (A) 10 225 (B) 0 150 mA/mgPtRu 2 mA/cm -10 75 -20 0 -30 PtRu/C4 -75 PtRu/C4 -40 -150 -0.4 -0.2 0.0 0.2 0.4 0.6 0.8 1.0 1.2 -0.4 -0.2 0.0 0.2 0.4 0.6 0.8 1.0 1.2 10 225 0 150 2 mA/mgPtRu mA/cm -10 75 -20 0 -30 PtRu/C2 -75 PtRu/C2 -40 -150 -0.4 -0.2 0.0 0.2 0.4 0.6 0.8 1.0 1.2 -0.4 -0.2 0.0 0.2 0.4 0.6 0.8 1.0 1.2 10 225 0 150 2 mA/cm mA/mgPtRu -10 75 -20 0 -30 PtRu/C1 -75 PtRu/C1 -40 -150 -0.4 -0.2 0.0 0.2 0.4 0.6 0.8 1.0 1.2 -0.4 -0.2 0.0 0.2 0.4 0.6 0.8 1.0 1.2 P o t e n t i a l (V) vs. S C E P o t e n t i a l (V) vs. S C EFigure 4. Cyclic voltammograms for PtRu/C electrocatalysts in 1M H2SO4 (column, A) and 0.5M CH3OH/1M H2SO4 (column, B) (scan rate 100 mV/sec). For methanol electro-oxidation potential peaks, PtRu/C2 showed lower peak potential amongall catalysts which indicate that this catalyst has good electrocatalytic activity for methanolelectrooxidation. On the other side, PtRu/C4 showed higher peak potential which could be attributed tothe presence of large agglomeration in this catalyst that could retard the oxidation of methanol at lowerpotential. The peak potentials for methanol oxidation on the catalysts prepared in this work are very
Int. J. Electrochem. Sci., Vol. 6, 2011 391closed to the peak potential for methanol oxidation on PtRu supported on acid functionalized carbonnanotubes (PtRu/CNTs) reported by Chetty et.al.and prepared by impregnation in ethanol followed byreduction at high temperature with flow of hydrogen and helium. To test the durability and stability of electrode catalysts to be applicable in DMFCs, allelectrodes were cycled in methanol for 100 cycles of potential sweep. The MAS activities for allelectrodes against cycle number of potential sweep are plotted in Fig (5). PtRu/C1 showed a decay forMSA and it decreases rapidly with increasing the cycle number. On the other hand for other electrodes,the MSA activities start low but increases with cycling, which is an indication that the cycling processactivates the electrode for methanol oxidation by adsorption of more methanol molecules and then theMSA is extremely stabilized. From Fig (5) we can detect that PtRu/C2 has higher MSA and goodstability, which futures this catalyst to be a promising catalyst electrode for methanol electro-oxidationin DMFCs. 260 PtRu/C1 240 PtRu/C2 220 PtRu/C4 200 MSA (mCmg ) 180 -1 160 140 120 100 80 60 40 0 10 20 30 40 50 60 70 80 90 100 110 Cycle NumberFigure 5. The MSA activities for PtRu/C catalysts electrodes as function of cycle number of potential sweep in 0.5M CH3OH/1M H2SO4.4. CONCLUSIONS The carbon supported PtRu nanocatalysts have been synthesized using a simple impregnationreduction method in ethanol as solvent and reducing agent at the same time. The XRD characterizationshowed that all catalysts exhibit f.c.c structure phase and only Ru h.c.p structure phase can be detectedat higher reaction time. From lattice constant calculations, the prepared catalysts are present inunalloyed form.
Int. J. Electrochem. Sci., Vol. 6, 2011 392 The PtRu nanoparticles showed a good dispersion on the support and the average particle sizewas in range of 3.7 nm with narrow particles distribution for PtRu/C prepared at 2h (PtRu/C2). Theelectrocatalytic activities of nanocatalysts evaluated in terms of mass specific activity. Among allcatalysts, PtRu/C2 showed higher electrocatalytic activity for methanol electro-oxidation. This workindicate how the reaction time and therefore the morphological feature influence the electrocatalyticactivity despite that all catalysts almost have the same crystal structure and the particle size. Anoptimum reaction time of 2h was able to produce nanoparticles with good dispersion and narrowparticle size distribution which enhance the catalytic activity. The work demonstrates that ethanolimpregnation reduction method is simple and low cost method for preparation of nanocatalysts aspromising materials for application in direct methanol fuel cells.ACKNOWLEDGMENTSThe authors are provided thanks for Emanuele Serra and Elena Salernitano, ENEA, Casaccia ResearchCentre, for the FESEM analyses and for help during the work. One of the authors, Abu Bakr A.A.Nassr is grateful thanks for Abdus Salam International Centre for Theoretical Physics (ICTP) andInternational Italian Agency for New Technologies; Energy and Environment (ENEA) for (ICTP-ENEA) fellowship on Training and Research in Italian Laboratories programme (TRIL- programme).References1. E. L. Gyenge, Chapter 4: Electrocatalytic oxidation of methanol, ethanol and formic acid’, in PEM Fuel Cell Electrocatalysts and Catalyst Layers, editor; Jiujun Zhang, Springer, New York, p. 165-270 (2008).2. A. O. Neto, R. W. R. Verjulio-Silva, M. Linardi and E.V. Spinacé, Int. J. Electrochem. Sci., 4 (2009) 954.3. A. B. Kashyout, A. A. A. Nasr, M. S. Mohy Eldin , Alexandria Engineering Journal, 48 (2009) 491.4. G.T. Burstein, C.J. Barnett, A.R. Kucernak, K.R. Williams; Catal. Today 38 (1997) 425.5. T. Iwasita, Electrochim. Acta 47 (2002) 3663.6. M. Brandalise, M. M. Tusi, R. M. Piasentin, M. Linardi, E.V. Spinacé, A. O. Neto, Int. J. Electrochem. Sci., 5 (2010) 39.7. H. Liu, C. Song, L. Zhang , J. Zhang, H. Wang, D.P. Wilkinson; J. Power Sources 155 (2006) 95.8. W. M. Martínez, T. T. Thompson, M. A. Smit, Int. J. Electrochem. Sci., 5 (2010) 931.9. A. Hamnett; Catal. Today 38 (1997) 445.10. J.L. Go´mez de la Fuente, M.V. Martı´nez-Huerta, S. Rojas, P. Terreros, J.L.G. Fierro, M.A. Pena; Catal. Today 116 (2006) 442.11. E.A. Bagotski, Y.B. Vassiliev, O.A. Khazova, J. Electroanal. Chem. 81 (1977) 229.12. G. Stalnionis , L. Tamasauskaite-Tamasiunaite , V. Pautieniene , A. Sudavicius, Z. Jusys, J. Solid State Electrochem. 8 (2004) 892.13. B. Gurau, R.Viswanathan, R.Liu, T.J. Lafrenz, K.L. Ley, and E. S. Smotkin, E.Reddington, A.Sapienza, B.C. Chan, T.E. Mallouk, S. Sarangapani, J. Phys. Chem. B 102(1998) 9997.14. Z. Liu, J.Y. Lee, W. Chen, M. Han, L.M. Gan, Langmuir 20(2004) 181.15. T. Maiyalagan Int. J. Hyd. Energy. 34 (2009) 2874.16. T. Maiyalagan, J Solid State Electrochem 13 (2009) 1561.17. S. Jingyu, H. Tianshu, C. Yanxia, Z. Xiaogang, Int. J. Electrochem. Sci. 2 (2007) 64.18. A.O. Neto, R.R. Dias, M.M. Tusi , M. Linardi, E.V. Spinacé, J. Power Sources 166(2007) 87.